DOI: 10.17188/1745574
title: Materials Data on Li32Mn11Cr5O48 by Materials Project

description: Li32Cr5Mn11O48 is beta Polonium-derived structured and crystallizes in the monoclinic C2 space group. The structure is three-dimensional. there are seventeen inequivalent Li sites. In the first Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–10°. There are a spread of Li–O bond distances ranging from 2.06–2.21 Å. In the second Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Li–O bond distances ranging from 2.04–2.21 Å. In the third Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.07–2.14 Å. In the fourth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Li–O bond distances ranging from 2.03–2.20 Å. In the fifth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.07–2.12 Å. In the sixth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Li–O bond distances ranging from 2.04–2.20 Å. In the seventh Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are four shorter (2.09 Å) and two longer (2.11 Å) Li–O bond lengths. In the eighth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two CrO6 octahedra, corners with two MnO6 octahedra, edges with two CrO6 octahedra, edges with two MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–9°. There are a spread of Li–O bond distances ranging from 2.05–2.21 Å. In the ninth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two CrO6 octahedra, corners with two MnO6 octahedra, edges with two CrO6 octahedra, edges with two MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Li–O bond distances ranging from 2.03–2.20 Å. In the tenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.06–2.21 Å. In the eleventh Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are four shorter (2.09 Å) and two longer (2.11 Å) Li–O bond lengths. In the twelfth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.07–2.22 Å. In the thirteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.06–2.22 Å. In the fourteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.06–2.21 Å. In the fifteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.07–2.21 Å. In the sixteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two CrO6 octahedra, corners with two MnO6 octahedra, edges with two CrO6 octahedra, edges with two MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.06–2.19 Å. In the seventeenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.07–2.12 Å. There are three inequivalent Cr sites. In the first Cr site, Cr is bonded to six O atoms to form CrO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Cr–O bond distances ranging from 1.90–1.98 Å. In the second Cr site, Cr is bonded to six O atoms to form CrO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Cr–O bond distances ranging from 1.91–1.99 Å. In the third Cr site, Cr is bonded to six O atoms to form CrO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 8°. There are a spread of Cr–O bond distances ranging from 1.90–1.98 Å. There are seven inequivalent Mn sites. In the first Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There is four shorter (1.94 Å) and two longer (1.95 Å) Mn–O bond length. In the second Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There is four shorter (1.94 Å) and two longer (1.95 Å) Mn–O bond length. In the third Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There is two shorter (1.93 Å) and four longer (1.95 Å) Mn–O bond length. In the fourth Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the fifth Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent CrO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There is two shorter (1.93 Å) and four longer (1.95 Å) Mn–O bond length. In the sixth Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There is two shorter (1.94 Å) and four longer (1.95 Å) Mn–O bond length. In the seventh Mn site, Mn is bonded to six O atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three equivalent MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There is two shorter (1.94 Å) and four longer (1.95 Å) Mn–O bond length. There are twenty-four inequivalent O sites. In the first O site, O is bonded to four Li, one Cr, and one Mn atom to form a mixture of edge and corner-sharing OLi4MnCr octahedra. The corner-sharing octahedra tilt angles range from 0–8°. In the second O site, O is bonded to four Li, one Cr, and one Mn atom to form a mixture of edge and corner-sharing OLi4MnCr octahedra. The corner-sharing octahedra tilt angles range from 1–8°. In the third O site, O is bonded to four Li and two Mn atoms to form a mixture of edge and corner-sharing OLi4Mn2 octahedra. The corner-sharing octahedra tilt angles range from 0–6°. In the fourth O site, O is bonded to four Li and two Mn atoms to form a mixture of edge and corner-sharing OLi4Mn2 octahedra. The corner-sharing octahedra tilt angles range from 0–8°. In the fifth O site, O is bonded to four Li, one Cr, and one Mn atom to form a mixture of edge and corner-sharing OLi4MnCr octahedra. The corner-sharing octahedra tilt angles range from 1–8°. In the sixth O site, O is bonded to four Li and two Mn atoms to form a mixture of edge and corner-sharing OLi4Mn2 octahedra. The corner-sharing octahedra tilt angles range from 0–6°. In the seventh O site, O is bonded to four Li and two Mn atoms to form a mixture of edge and corner-sharing OLi4Mn2 octahedra. The corner-sharing octahedra tilt angles range from 0–6°. In the eighth O site, O is bonded to four Li, one Cr, and one Mn atom to form a mixture of edge and corner-sharing OLi4MnCr octahedra. The corner-sharing octahedra tilt angles range from 0–8°. In the ninth O site, O is bonded to four Li, one Cr, and one Mn atom to form a mixture of edge a